10 POLIMERY 2001, 46, nr 1
JULITA JAKUBIAK* * ***)1, JAN F. RABEK" 1
Modeling of the kinetics of linear and crosslinking
photopolymerization. Part III****
Summary — A review with 135 references continuing the comparison
of modeling of linear and crosslinking photopolymerizations and
covering the gel formation during crosslinking, the gel effect
(autoacceleration of polymerization), modeling of the overall rate
of polymerization, the rate of polymerization in the photoinduced
electron/proton transfer mechanism, the kinetic treatment of
photopolymerization by photo-differential (isothermal) scanning
calorimetry, and reactivities of radicals and monomers.Key words:
photopolymerization, photoinitiators, kinetics of initiation,
propagation and termination steps.
GEL FORMATION DURING CROSSLINKING
Photopolymerization of monomers with the functionality higher
than 2 produces a branched polymer (Fig. la). The growing branches
interact with each other to produce infinite molecular weight
Fig. 1. Schematic presentation of: (a) branched macromolecule
(pregel state) and (b) crosslinked net
products (Fig. 2b) known as gels. Since multifunctional monomers
have more than one functional group, each group may possess a
different reactivity. In general, this functional group reactivity
is not only unequal but it also varies with the degree of
conversion of the double bonds in the system. Any polymerization
involving multifunctional monomers has this added complexity of
possibly varying reactivity of functional groups on
*) Jagiellonian University, Department of Chemistry, Ingardena
3, 30-060 Cracow, Poland. To whom all correspondence should by
” ) Polymer Research Group, Department of Dental Biomateriał
Science, Karolińska Institute (Royal Academy of Medicine), Box
4064,141 04 Huddinge (Stockholm), Sweden.
***) For Part II see .
the same molecule, what causes structural heterogeneity [2, 3].
The primary result is the formation of microgel regions early in
the reaction, because of high pendant double-bond reactivity [4—
8]. Microgels are regions in the system of higher average
crosslinking density than that of the overall system, manifested
from the strong spatial correlation between pendant group
reactivity and radical location . Usually, the crosslinking
Fig. 2. Schematic presentation o f a microgel 
photopolymerization forms densely crosslinked microgel regions
within a less densely crosslinked area (Fig.2). The microgel
regions are formed near the radical initiation sites. It has also
been observed that, in the same polymer network, unreacted monomer
pools can exist [7, 8]. This heterogeneity not only affects the
reactivity of monomeric and pendant functional groups, but it also
affects the material properties . A heterogeneous material may
have properties which are dramati-
CORE Metadata, citation and similar papers at core.ac.uk
Provided by Jagiellonian Univeristy Repository
POLIMERY 2001, 46, nr 1 11
cally different from the properties of the corresponding
homogeneous material [11— 15]. The resulting polymer structures are
often extremely difficult to characterize either experimentally
When a radical on a polymer chain propagates through a pendant
double (i.e. a double bond from a monomer with one double bond that
has already reacted), primary cycles, crosslinks and secondary
cycles can be formed (Fig. 3) [3, 16, 17]:
Fig. 3. Classification of the reactions o f pendant double bonds
during free radical crosslinking polymerizations 
■— primary intramolecular cycles result, when propagating
radicals react with pendant double bonds on their own kinetic
— intramolecular crosslinks form when the radicals react with
pendant double bonds on different kinetic chains;
— secondary intramolecular cycles result when propagating
radicals react with pendant double bonds on different kinetic
chains with which they are already
crosslinked. As the chain flexibility increases, the
reactivities of the pendant functional groups are enhanced what
leads to extensive cyclization at a low conversion [18—21].
Fig. 4. Kinetic gelation model prediction o f the relative
fraction o f crosslinks, and primary and secondary cycles as a
function o f double bond conversion in the polymerization of a
multifunctional monomer 
In Fig. 4. are shown the relative fractions of crosslinks, the
primary and secondary cycles as a function of double bond
conversion for homopolymerization of a tetrafunctional monomer .
Initially, primary cyclization dominates crosslinking and secondary
cyclization, as the pendant double bonds have an increased
reactivity in the localized region of the free radicals. This
behavior accounts for the formation of microgel regions and the
heterogeneity of the network. As the conversion and the polymer
concentration increase, crosslinking and secondary cyclization
begin to increase and a network forms. Finally, a transition region
is reached where secondary cyclization and primary cyclization
cross over. The trend is now towards a more homogeneous network
structure with a very high degree of secondary cyclization .
For cyclization to occur, the propagating radical and pendant
double bond, attached to the same molecule, need to come into a
small reactive volume of the order of Angstroms in size . At
low conversions (
12 POLIMERY 2001, 46, nr 1
the cyclization rate . The rate of consumption of pendant
double bonds by crosslinking is analogous to the rate expression
for the consumption of monomeric double bonds (cf. ).
Crosslinking is the function of the kinetic parameter for
crosslinking, the concentration of pendant double bonds, and the
concentration of radicals in a polymerizing system. The rate of
cyclization depends on the kinetic parameter for cyclization, the
pendant double bond concentration, and the local radical
concentration. The expression is summed over all times in which the
pendant groups were created, since the local concentration depends
on when the pendant group was created and how far the radical on
the same chain has propagated away. The local propagation radical
concentration (at time t that have reacted between the radical (R")
and monomeric double bond that
Fig. 5. Local radical concentration versus (t-tb) 
react to form the pendant group birth at time tb) (Fig. 5) is
given by the equation:
1( 1 )
where: NA is the Avogadro number, and r is the radius containing
the local radical for a particular pendant group (Fig. 6) given
Г = re_' + r0 (2)where: re.c is the average end-to-end distance
and r0 is the di-
Fig. 6. The radius containing the local radical for a particular
pendant group 
stance between double bonds. The is given by the equation:
7rc - c = l M n h , (3)
where: lM is the effective monomer size and n, , is the number o
f repeat units added since the pendant groups formed and given by
t4.h = I Л dt (4)
where: r| is the propagation factor.
The rate of the overall consumption for pendant groups
consumption (Rpcn) is given as :
Rpn, = крс„[РЕЩ Г]+ & суДРИПл [РЧ,„ (5)/„=0
where: kpm is the rate constant o f pendant groups formation,
[Рш] is the concentration o f propagating radicals, given as (cf.
 eqn. (6)):
[P‘ ] =4 k> ,
where: f is the photoinitiator efficiency, kd and k, are rate
constants of the photoinitiator decomposition and termination,
respectively, [I] is the photoinitiator concentration; [PEN] is the
pendant group concentration in a monomer, [PEN],, (at time t that
have reacted between the radical (R')and monomeric double bond that
react to form the pendant at time tb), kcyc is the rate constant
for cyclization, can be assumed to be the same as the rate for
ką/c = kp (7)
however, kclJC is lower than the kp due to the mobility
limitation of pendant groups composed to monomer. The kcyc is by
two orders of magnitude lower than the kp. This reduction is
approximately equivalent to the reduction in the kp of 80%
conversion due to diffusion induced mobility limitations, i.e.:
к cyc ^ kp (8)The complete expression for the local radical
tration ([P* ]) is :
[P'U exp(-fc,[P’](f- f j)1
f ( 1 >3\N ,
4j k r0 + r>uJM
This calculation assumes a spherical-shaped molecule with the
double bonds on the radius.
AUTOACCELERATION OF POLYMERIZATION (GEL EFFECT)
An autoacceleration process (also known as the gel effect or as
the Trommsdorff effect ) is observed to occur both in linear
and crosslinking polymerizations, due to a decrease of the
termination rate constant (к,) at
POLIMERY 2001, 46, nr 1 13
higher monomer conversions [25, 26]. When the polymer
concentrations grow, the macroradicals will become entangled with
segments of other polymer chains and formed polymer nets. As a
result, the rate of diffusion of the propagating radicals and the
frequency of their mutual encounters will decrease, and k, is
reduced. In linear polymerization, the decrease of kt occurs slowly
at 30—50% of monomer conversion and then rapidly (at 70—80%)
[27—30]. The termination process proceeds by two mechanisms: one
controlled by segmental diffusion at low conversions (independent
of chain length), and another controlled by translational diffusion
after the gel effect has started (dependent on chain length) [3,
26, 27, 31, 32]. Rate constants кл and kp are independent from
growing propagating radicals at low conversions, and remain
constant with concentration, until high concentrations are achieved
where the polymerizing system begins to exhibit glassy effects [33,
34]. The initiator efficiency (f) may change by a factor of ~2
prior to the onset of the glass effect [34, 35]. Defining К
K = k, AKk,
all of the change in К is due to variation in kt over all the
conversion range. Generally, the propagation rate constant (kp)
remains almost constant over a wide conversion range, whereas the
termination rate constant (kt) decreases with conversion showing a
plateau at the middle of the conversion region (Fig. 7). In this
region, kt be-
Double bond conversion
Fig. 7. The characteristic behavior o f the propagation (kp) and
termination (k f rate constants as a function of double bond
conversion for multifunctional monomer crosslinking polymerization
comes proportional to fcp[M] due to the dominance of a reaction
diffusion termination mechanism [26,36]. Diffusion of very long,
entangled chains has a stronger concentration dependence than that
of untangled chains. Termination related to the gel effect is not
controlled by the chain-end segmental mobility but, instead, is
controlled by diffusion of the shortest propagating radical
chains. This gives credence to the proposals of "short-long"
termination processes [37—39] in which short propagating radical
chains control the termination reaction. An approach to this
problem is to compare data on the termination rate constant (k,)
with diffusion data in order to determine the type of diffusion
control termination [3, 36, 40— 47].
In the crosslinking polymerization k, is strongly dependent on
the size of the radicals involved in the termination reaction. The
termination reaction is diffusion controlled from the beginning of
polymerization and the diffusivity of propagating radicals is
dependent on chain length [48—50]. In the crosslinking
polymerization termination reactions occur between relatively large
propagating radicals entangled in the growing polymer net, and
termination rates are limited by the rates at which the radical
ends can encounter with each other [51—53]. As a result, kt is a
decreasing function of the size of the propagating radical. The
segmental diffusion coefficient and the termination rate constant
(k,) increase as the polymer concentration increases from zero.
In the modeling of diffusion controlled kinetics, the
polymerization rate constant (крЫф) and the termination rate
constant (k,M№) which combines a term for the translation/segmental
diffusion and the reaction diffusion, are [51, 54]:
1 1( И )
-------------- + --------------
K p(chcm )
]r 4_ Ł*л7(Гл»к/*у) ^ л/ ( ж / ) ( 1 2 )
where: kp(Mdî is the rate constant for monomer diffusion,
Aim,,) is the rate constant for chemical reaction, kl(lrims/sê is
the termination rate constant for translation/segmental diffusion,
and kHrmc0 is the termination rate constant for reaction
The кШф for crosslinked polymerization can be derived from
Smoluchowski's equation for the prediction of diffusion controlled
bimolecular rate coefficients  and Einstein's relation between
the diffusion coefficient and the frequency of propagation [8, 56,
W ) = y ^ 2r. W (13)
where: f is the probability o f reaction when two radicals come
within the capture distance o f each other, a is the
root-mean-square end-to-end distance per square root o f the number
o f monomer units, and r„ is the radius o f interaction at two
— at rigid limit: the chain end cannot move on the time scale o
f propagation, and thus, the radius o f interaction is half the
diameter of monomer (
14 POLIMERY 2001, 46, nr 1
1 at high conversion, Ę, - 0.25 at low conversion, and Ę, = 0 in
sterically hindered systems) [57, 59].
Two diffusion controlled termination rates, minimum (Riidifflmn)
and maximum (RtUiJf)m J , are given by the equations [35, 46,
(d if f) min
''t(d iff) max_ 4Л j. 3 -2
kp[M] 3 (15)
R,(dlp for acrylates is 3—5 liter • mol"1  and for
methacrylates is 2 liter • mol"1 . The ratio of:
R ( d i/ n max
R t ( d i f f ) min
= 2(1 - (16)
Since the ratio (a /a ) is of the order of 1 and j approaches 1
as the crosslinking density increases, Rl(dlig) approaches 2 for a
highly crosslinked polymer matrix . For a loosely crosslinked
network, polymerized above the glass transition temperature (Tg),
Rt(dip should approach the flexible limit, i.e. because the
distance from the last attachment to the network is significantly
larger, and the overall mobility of the system is increased by
polymerizing above Tg. As the polymerization temperature is lowered
below T , the distance back to the last network attachment point or
entanglement becomes less important, and the mobility of the
radical chain end is reduced to the point where it is virtually
immobile on the time scale of propagation. In this case, the rigid
limit should be applicable, and RtUip should approach К,мда„„„,
just as it would for a highly crosslinked network .
Deviations resulting from the diffusion control of termination
at low conversion of monomer (
POLIMERY 2001, 46, nr 1 15
Irradiation time, s
Fig. 8 . Two rates o f polymerization of: (a) triethylene glycol
dimethacrylate (TEGDM) and (b) TEGDM and poly(acrylic acid), both
in air [71, 72]
gels . Another explanation of the two peak maxima observed
in photopolymerization in air was proposed on the basis of
different reactivities of propagating radicals and peroxy and oxy
radicals [69, 71—75]:
P’ + 0 2------ > POO" (23)
POO' + PH------ > POOH + P’ (24)
Very reactive oxy (PO‘) radicals are formed by thermal
decomposition of hydroperoxy groups (POOH) by the heat of
POOH — £-> PO‘ +'OH (25)
In a number of photopolymerizations there is observed a postcure
effect, which is a light-independent polymerization occurring after
light has been switched off. The postcure effect can be explained
by that the residual unreacted initiator generates sufficient
amounts of radicals to promote crosslinking regardless of the
greater immobility of the network.
MODELING OF OVERALL RATE OF POLYMERIZATION
Modeling of the overall rate of polymerization (initiation,
propagation and termination) requires an accurate
reaction kinetic model to predict the rate of polymerization at
a given temperature and conversion. The kinetic model should
— photoinitiator concentration and efficiency, mechanism and
kinetics of a photoinitiator decomposition into free radicals,
radicals reactivity and selectivity in the initiation of
propagation, inhibitor concentration and kinetics of inhibition,
the effect of temperature;
— the acceleration and deceleration of propagation reaction due
to gel effect and diffusion limitations;
— termination of propagation due to recombination reactions,
chain transfer and trapping of propagation radicals in a polymer
— the kinetics of conversion and final extent of cure;— volume
contraction (shrinkage).Several models have been developed to
toacceleration in the absence of a significant delay in volume
shrinkage for linear polymerization [76—81].
The following equations have been used for modeling the linear
polymerization with V as system volume :
Id[MV] = - ^ [M]£ r i i V a t „=[ (26)
l ^ P = 2 fkJ[I]-k,[M][R-]V dr
1 d[lv]= - mV dt d (28)
i d [p -v u = k m [ R . j_ *дМ][р. L _ _ [P- L , 2 к ,Г ]„ v at
= ~k>'[Mt [P' - [p' Ł) - [ r 1. £ м р‘ l (30)
where: [I] and [M] are concentrations o f initiator and monomer,
respectively, [R'] is the concentration o f radicals from the
initiator decomposition, [P’]„ is the concentration of the
propagating radical o f length n , f is the initiator efficiency,
kd, k, and kp are rate constants o f initiator decomposition,
initiation o f polymerization, and propagation, respectively, and t
is the polymerization time.
For further modeling, eqns. (30) and (31) can be reduced to
dt 1 +mp ,l=] (31)
d Z n (2>ч1 z . v~ j T = -------- a -p )* , + 2 fkAi]-k,\ Z
lP ’Ldt 1+Ш P ) (33)
where: со is a volume contraction factor defined as:
ns- Am ~dp (34)V
where: dM and dP are monomer and polymer densities,
respectively, and p is the fractional monomer conversion.
16 POLIMERY 2001, 46, nr 1
With appropriate information about the initial values of the
rate parameters and their dependencies on system conditions, eqns.
(32—33) can be solved simultaneously by using numerical techniques
to provide predicted conversion-time results.
The rate of polymerization is difficult to model because of the
competing reactions between several photoinitiators, inhibitors,
and comonomers [82, 83], changing initiator efficiency ,
effects of free volume [26, 66, 85, 86], homegeneities during
network formation , entanglements , substitution effects
[89—91], diffusion limitations [83, 84, 92—94], gel inhomogeneities
before gel point [92, 96], reactions between microgel particles
after the gel point , simultaneous crosslinking and scission
reactions , and a delay in volume shrinkage and incomplete
conversion of reactive groups [2 ].
Assumption of a steady state is valid only for linear
polymerization of monofunctional monomers and polymerization in
solution; however, it does not apply to the photocrosslinked
polymerization . The reason is that the low mobility of
propagating radicals causes that termination by radical
recombination is not a significant factor as in the case of
conventional polymerization of monofunctional monomers. The
analytical solution of the kinetic equations becomes difficult in
the absence of the steady-state condition. Much effort has been
spent in order to model crosslinking polymerization through [3,
— statistical approach, whereby polymer structures evolve
according to certain probabilistic rules for the formation of bonds
between smaller monomer molecules [100— 107].
— kinetically based approach, which involves solving the
differential equations that describe the concentration of each
reacting species [67, 108— 115].
— structure simulation approach, which involves simulation of
the structure in space using a percolation type simulation called
the kinetic gelation model [9,116—123].
RATE OF POLYMERIZATION IN THE PHOTOINDUCED ELECTRON/PROTON
TRANSFER (EPT) MECHANISM
With the steady state assumed to occur, the rate of donor
radicals (D‘) production is equal to the rate of radicals D'
termination by the combination process:
R d. = R/c at steady state conditions (38)
Substituting eqns. (40) (cf. , eqn. (57))
RD. = ^ P = k,I„lDH] (39)
where (cf. , eqn. (16))
h = Io c [ l] l (40)
where: I„ is the intensity o f the light absorbed, I0 is the
intensity of incident light, s is the molar extinction and l is the
path length, and eqn. (42) (c f , eqn. (70))
R lc = 2klc [ D f (41)
into eqn. (39) gives
K, I„ [DH] = 2ktc [D-]2 (42)
where: klc is the rate o f termination o f radicals D' by the
D ’ + D ' — ——> inactive products (43)
D ’ + M ‘ — > inactive products (44)
The overall termination rate constant by recombination is:
К ~ кict + klc2 (45)
[D'] =K th lD H ]
Substituting eqn. (46) into eqn. (37), the rate of
polymerization (Rp) is
'y ,[P H ]V2 k „ .
Combination of eqn. (48) (cf. , eqn. (37)):-AG#''кы = kZ
Donor radicals (D") formed in the reaction [eqn. (35)] (cf.
, eqn. (53)):
I*+DH-----> IH' + D ' (35)
where: I is the initiator and DH is the donor molecule.
The donor radical (D‘) initiates polymerization reaction:
D ' + M - (36)
The rate of polymerization (Rp) for the bimolecular reaction
 is given by:
Rr=-d[M] кd t
where: к is the electronic transition coefficient, Z is the
nuclear frequency factor, AG# is the free energy o f activation,
and eqn. (49) (cf. , eqn. (38)):
where: X is the reorganization energy and AG° is the free
enthalpy, with eqn. (47) gives:
kZ exp4 Ю]
LID H ]RT 2 K
POLIMERY 2001, 46, nr 1 17
Equation (50) shows that the rate of polymerization (Rp) in the
EPT process depends on the thermodynamical parameter AG°. The rate
constant of polymerization (Rp) should increase with decreasing AG°
at relatively high values of AG°, whereas it should decrease with
increasing AG° at low values of AG° (i.e., AG° is negative and
large). The region where Rp decreases with decreasing AG° is called
the Marcus "Inverted Region". The parabolic (bell) shape of the
Marcus plot (Fig. 9) shows that the Rp depends considerably on the
structure of hy-
No. N-substi- tuent R2p-substi- tuent R,
Eox, mV AG°, eV
1 H H 426 -0.485
2 H NO 707 -0.204
3 H NOj 781 -0,130
4 H 0II
H3C -C —
5 H 0II
P h-C —
6 H 0II
7 H Cl 479 -0,432
8 H CH„ butyl 437 -0,474
9 H tert-Bu 436 -0,475
10 H PhO 479 -0,432
11 H MeO 343 -0,568
Fig. 9. Rate o f polymerization (Rp) as a function of the free
energy o f activation (AG°) for camphorquinone (I) and differently
substituted N-phenyl glycines (1— 10) (results give the Marcus
parabolic relation) 
drogen atom donors (DH), i.e., on their oxidation potentials
(Eor(DH/DH'+). The Rp values calculated from eqn. (50) are valid
only for linear polymerization, because of the steady state
assumption. Nevertheless, this kinetics has been applied to
KINETIC TREATM EN T OF PHOTOPOLYM ERIZATION BY
PHOTO-DIFFERENTIAL (ISOTHERMAL) SCANNING
Photo-differential (isothermal) scanning calorimetry (photo-DSC)
has been extensively used for the study of crosslinking
photopolymerization [125,126]. An isothermal DSC trace is a plot of
the heat evolved in polymerization reaction against the time of
reaction; it allows to determine several kinetic parameters (Fig.
10): the rate
Lnh W x Irradiation time, s
Fig. 10. Typical DSC photopolymerization profiles and
indications o f the: rate o f polymerization (Rp and Rpmax), time
to reach the maximum rate o f polymerization (t„mx), inhibition
time (tinh) (from the slope o f kinetic curve crossing the
coordination o f irradiation), double bond conversion (p), its
maximum (pm„x) and p at Rp'""1
of polymerization (Rp), the maximum rate of polymerization
(Rpmax), the double bond conversion (p), the highest degree of
double bond conversion (pmax), the time in which Rp™1 appears
(tmlx), inhibition time (f,Wj), Rp versus p (Fig. 11), inhibition
and retardation kinetics (Fig. 12), reaction order, activation
energy, and Arrhenius preexponential factor. A most general
treatment of thermo- analytical kinetic data gives very condensed
accounts of the isothermal DSC method . The fact that typical
photo DSC samples («1 mg) are around 80 microns thick led to one of
the biggest problems in the methodi-
18 POLIMERY 2001, 46, nr 1
Double bond conversion
Fig. 22. A typical rate o f polymerization (Rp) versus
conversion o f double bonds conversion (p)
Considering the Avrami rate law [130—132], the rate of
polymerization (Rp) can be presented as
d t = к т(52)
RP= - ^ L = kl,\Mm i (53)
where: P is the dead polymer, and n and m are integers.
[M ],= [M L (l-a ) (54)
where: a is the fraction o fM reacted at time t, eqn. (53)
= [Ml ^ = fc,[MEa-a)" (55)
Fig. 12. Conversion versus time plots for normal, retarded and
cal development of this technique, the extent of light
absorption through the sample. This film thickness makes photo DSC
well-suited to the study of propagation kinetics in thin films but
far removed from the conditions of kinetics polymerization in the
bulk. The self-screening (c f ) that occurs in the samples also
shows itself as an exotherm distortion . The isothermal DSC
trace is distorted to have a steep leading edge (indicative of the
very fast photopolymerization at the sample surface), and a long
trailing back edge (indicative of the low probability of light
absorption by the photoinitiating system near the bottom of the
The instantaneous heat release (AH,) at a given time (f), (the
DSC ordinate y) at time t is proportional to the rate of
polymerization (Rp) at that time t, i.e., to -d[M]/dt:
dA H,d[M], = df
Fig. 13. Kinetic curves for reactions conforming to eqn. (52),
for: (a) n = 0, (b) n = 1/2, (c) n = 1, (d) n = 3/2 and (e) n = 2
where: A H0 is the theoretical enthalpy o f polymerization, and
Fig. 14. Kinetic curves for reactions conforming to eqn. n is the
number o f double bonds present in a monomer; eg ., (53), for: (a)
n = m = 2/2, (b) n = m = 1, (c) n = m = 3/2(AH0 = 57 800 J • mol'1
for the methacrylate group ). and (d) n = m = 2 
POLIMERY 2001, 46, nr 1 19
^ = /(а) = /сДМГ(1-°0" (56)dc
Modeling these equations with n = 0, n - m = 1/2, 1, 3/2 and 2,
gives the kinetic curves shown in Fig. 13 and Fig. 14 .
REACTIVITIES OF RADICALS A N D M ONOM ERS
Reactivities of various radicals are usually assessed by
comparing the rate constants for selected reactions. This is not a
convenient procedure in free-radical crosslinking polymerization,
because absolute rate constant measurements are still not
available. However, the relative reactivities of various monomers
towards a given radical can be computed from the reciprocals of the
reactivity ratios. It is not possible to conclude that R,' will
always react x times more rapidly than radical R f in addition
reactions or у times as rapidly in the hydrogen-atom absorption
reactions. This is because resonance, steric, and polar influences
all come into play and their effects can depend on the particular
species involved in a reaction. Understanding of how resonance,
steric, polar and electronic factors influence radical-monomer
reaction rates is far from complete [134, 135].
The controlling factor in the reactivity of a given monomer is
the stability of the radical (P*) formed by addition of the monomer
(M) to the initial radical (R’). Monomers that yield radicals in
which the unpaired electron is extensively delocalized have ground
state structures that are themselves resonance stabilized. The
important factor is the relative stability of the radical (P‘),
because a single unpaired electron is more easily delocalized than
one in the C=C double bond. Thus, the resonance stabilization
causes an increase in monomer reactivity and a decrease in the
reactivity of the propagating polymer radical.
Free radicals formed from photoinitiators by a-pho- tocleavage
 and by hydrogen-atom transfer  and multifunctional
monomers are neutral, but variations in the reactivities of all
these species can be rationalized and predicted by considering that
the transition states in their reactions may have some polar
effects. Appropriate substituents may facilitate or hinder a
particular reaction because of their influence on the polarity of
the reaction site.
The effect of substituents on the relative radical efficiency
(f)  is expressed by the Hammett equation [137, 138]:
— = рст+ R + E sfo
where: / and f 0 are radical efficiency with a substituent S in
place, and reference radical with hydrogen atom as a substituent at
the same position, respectively; p is the substituent constant and
is a measure o f the electronic effect o f the substituent S at the
particular position; a is the reaction constant
which measures the sensitivity o f the reaction to the
electronic effect o f a substituent at a particular position in the
molecular framework; R and Es are resonance and steric effects,
The resonance (R) and steric effect (Es) can be neglected. If a
plot of log(f//0) versus a (at а = 1) gives a straight line which
passes through the origin (0,0), a linear Hammett correlation is
obtained (Fig. 15). A linear correlation tells us that the radical
efficiency is affected in a consistent way by the electron donating
or withdrawing ability of substituents (S). A positive p means that
the radical efficiency increases with electron withdra-
Fig. 15. Plot o f relative radical reactivity [log (f/f0) 1
versus Hammett substituent parameter (a) 
wing substituents. Conversely, a negative p indicates that the
radical efficiency is favored by electron donating substituents
The effects of substituents on the reactions on phenyl rings
permit the assignment of nucleophilic (electron-releasing)
character to various groups . These include alkyls, vinyl,
hydroxyl, ether, phenyl and ester groups. Electrophilic (electron
withdrawing) substituents include halogen, nitro, cyanide,
carboxyl, and carbonyl groups. Steric influences may also retard
some radical polymerizations.
Kinetic model predictions of monomer reactivity can be evaluated
on the monomer mobility . The reactivity (R) of pendant
functional groups to monomeric functional groups can be determined
R = 2[M][P]
20 POLIMERY 2001, 46, nr 1
25% conversion, the reactivity of the pendant functional group
is significantly higher than that of the monomeric functional
group. This is expected as pendant functional groups exist only in
the local region around the active radical and are, therefore, much
more likely to react with it. As the reaction proceeds to higher
conversions, pendant functional groups become imbedded and trapped
within the polymer matrix, inaccessible to the active radicals.
This tendency decreases the effective concentration of pendant
functional groups and hence decreases the reactivity above a
conversion of approximately 70%, beyond which the reactivity ratio
falls below 1.0. The imbedding of functional groups, both monomeric
and pendant, within the polymer leads to the attainment of a
maximum conversion despite the presence of continuing initiation
Fig. 16. The reactivity ratio as a function o f conversion: (a)
a complete range o f reactivity ratios, (b) an expansion o f the
lower reactivity ratio regime 
Studies of the reactivities of different multifunctional
monomers are the subject of several publications [54, 125]. For
example, the rate of photopolymerization of triacrylates is higher
than that of diacrylates (Fig. 17), and that of
dimethacrylates higher than that of diacrylates . This trend is
as expected because an increase in the flexibility of the
OA 0.8 1.2 1.6 2.0Irradiation time, min
Fig. 17. Comparison o f the photocuring o f triacrylate and
diacrylate during continuous UV exposure 
group allows a greater level of reaction before the network is
formed. Monomers with pendant vinyl group exhibit a greater
mobility, and lead to a highest extent of polymerization
The kinetic model of gelation does not assume the functional
groups in multifunctional monomers to be equireactive, whereas in
contrast, the homogeneous model assumes equal reactivity of all
double bonds present in a monomer . In Fig. 18 is shown the
Conversion of functional groups
Fig. 18. Kinetic gelation model prediction
prediction for homogeneous and heterogeneous assumptions. For
example, at 50% conversion of the functional groups, the
homogeneous assumption predicts that 75%, whereas the heterogenous
predicts 69% of the monomer, has at least one double bond reacted
and is unextractable .
End note: This article has been written by Dr. Julita Jakubiak,
Head o f the joint project "Mechanisms, kinetics and applications
of photopolymerization initiated by visible light photoinitiators",
supervised by Prof. J. F. Rabek and Prof. J. P. Fouassier. Dr. J.
Jakubiak spent one year
POLIMERY 2001, 46, nr 1 21
(1998/1999) as post-doc researcher at Polymer Research Group,
Department o f Dental Biomateriał Science, Karolińska Institute,
The Royal Academy o f Medicine, Stockholm, Sweden (directed by Prof
J. F. Rabek) and one year (1999/2000) as post-doc researcher at the
Laboratoire de Photochimie Generale, CNRS, University o f Mulhouse,
France (directed by Prof. }. P. Fouassier).
[I] Jakubiak J., Rabek J. E: Polimery 2000, 45, 659. 
Kloosterboer J. G.: Adv. Polym. Sci. 1988, 84, 1.  Anseth K. S.,
Newman S. M., Bowman C. N.: Adv. Polym. Sci. 1995,122,179. 
Bastide J., Leibler L.: Macromolecules 1988, 21, 2647.  Funke
W.: Br. Polym. J. 1989, 21, 107.  Matsumoto A., Matsuo H., Ando
H., Oiwa M.: Eur. Polym. }. 1989, 25, 237.  Anseth K., Bowman
C.N., Peppas N. A.: ]. Polym. Sci. Chem. Ed. 1994, 32, 139.[8 ]
Anseth K. S., Anderson K. J., Bowman C. N.: Makro- mol. Chem. Phys.
1996, 197, 833.  Anseth K. S., Bowman C. N.: Chem. Eng. Sci.
1994, 49, 2207.  Dusek K. in: "Advances in Polymerization"
(ed., Flaward R. N.), Applied Science Publications, London
[II] Kannurpatti A. R., Anseth J. W., Bowman C. N.: Polymer
1998, 39, 2507.  Simon G. P, Allen P. E. M., Bennett D. J.,
Wiliams D. G. R., Wiliams E. FI.: Macromolecules 1989, 22, 3555.
 Wilson T. W.: }. Appl. Polym. Sci. 1990, 40, 1195.  Simon
G. P, Allen P. E. M., Williams D. R. G.: Polymer 1991, 32, 2577.
 Matsuoka S.: "Relaxation Phenomena in Polymers", Hanser
Publisher, New York 1992.  Dotson N. A., Macosco C.W., Tirrel
M. in: "Synthesis, Characterization and Theory of Polymeric Network
and Gels" (ed., Aharoni S. M.), Plenum Press, New York 1992, p.
319.  DusekK., MacKnight W. J. in: "Crosslinked Polymers,
Chemistry, Properties and Applications" (eds., Dickie R. A., Labana
S. S., Bauer R. S.), ACS Symposium Series, No. 367, American
Chemical Society, Washington, DC 1988, p. 2.  Dusek K., Ilavsky
M.: J. Polym. Sci. Polym. Symp. 1975, 53, 47 and 75.  Shah A. C
, Holdaway I., Parson I. W., Haward R. N.: Polymer 1978, 19, 1067.
 Matsumoto A., Matsuo H., Oiwa M.: Makromol. Chem. Rapid
Commun. 1987, 8, 373.
 Landin D. T., Macosko C. W.: Macromolecules 1988, 21, 846.
 Winnik M. A.: Acc. Chem. Res. 1985, 18, 73.  Gibson J. E.,
Anseth J. W., Bowman C. N.: Proc. Conf. RadTech '99, Berlin,
Germany 1999, p. 757.  Trommsdorff E., Kohle E., Lagally R:
Makromol. Chem. 1948, 1, 169.  O'Neil G. A., Torkelson J. M.:
Trends Polym. Sci. 1997, 5, 349.  O'Neil G. A., Torkelson J.
M.: Macromolecules 1999, 32, 411.  Soh S. K., Sundberg D. C.:
J. Polym. Sci. Chem. Ed. 1982, 20, 1315. Ballard M., Napper D.
FI., Gilbert R. G.: }. Polym. Sci. Chem. Ed. 1984, 22 , 320. 
Sack R., Schulz G. V., Meyerhoff G.: Macromolecules 1988, 21, 3345.
 Var- swell T. G., Hill D. J. T., Londero D. L, O'Donnell J.
H., Pomery P. J., Winzor C. L.: Polymer 1992, 23, 137.
 Soh S. K., Sundberg D. C : J. Polym. Sci. Chem. Ed. 1982,
20,1299.  O'Neil G. A., Wisnudel M. B., Torkelson J. M.: AIChE
J. 1998, 44, 1226.  Zhu S., Tian Y„ Hamielec A. E., Eaton D.
R.: Polymer 1990, 31, 154.  Parker H. Y., Westmoreland D. G.,
Chang H. R.: Macromolecules 1996, 29, 5119.  Russell G. T.,
Napper D.H., Gilbert R. G.: Macromolecules 1988, 21, 2141. 
Anseth K. S., Wang C. M., Bowman C. N.: Polymer 1994, 35, 3243.
 Russell G. T., Gilbert R. G., Napper D. H.: Macromolecules
1992, 25, 2459.  Russell G. T., Gilbert R.G., Napper D. H.:
Macromolecules 1993, 26, 3538.  O'Shaughnessy B., Yu J.:
Macromolecules 1994, 27, 5067 and 5079.  Stickler M.: Makromol.
Chem. 1983, 184, 2563.
 Anseth K. S., Wang C. M., Bowman C. N.: Macromolecules
1994, 27, 650.  Faldi A., Tirell M., Lodge T. R: Macromolecules
1994, 27, 4176.  Buback M., Huc- kestain B., Russell G. T.:
Makromol. Chem. Phys. 1994, 195, 539.  Anseth K. S., Kline L.
M., Walker T. A., Anderson K. J., Bowman C. N.: Macromolecules
1995, 28, 2491.  Mateo J. L., Serrano J., Bosch R:
Macromolecules 1997, 30, 1285.  Young J. S., Bowman C. N.:
Macromolecules 1999, 32, 6073.  Mateo J. L., Calvo M., Serrano
J., Bosch R: Macromolecules 1999, 32, 5243.  Cardenas J. N.,
O'Driscoll K. R: J. Polym. Sci., Chem. Ed. 1976, 14, 883. 
Cardenas J. N., O'Driscoll K. R: J. Polym. Sci., Chem. Ed. 1977,
15, 1883.  Soh S. K., Sundberg D. C.: J. Polym. Sci. Polym.
Chem. Ed. 1982, 20, 1299, 1315, 1331, 1345.
 Cook W. D.: Polymer 1992, 33, 2152.  Zhu S., Tian Y.,
Hamielec A. E., Eaton D. R.: Macromolecules 1990, 23, 1144. 
Okay O.: Polymer 1994, 35, 796.  Cook W. D.: ]. Polym. Sci.
Polym. Chem. Ed. 1993, 31, 1053.  Smoluchowski M.: Z. Phys.
Chem. 1918, 92, 129.  Russell G. T., Napper D. H., Gilbert R.
G.: Macromolecules 1988, 21, 2133.  Russell G. T., Gilbert
R.G., Napper D. H.: Macromolecules 1993, 26, 3538.  Flory P.
J.: "Statistical Mechanic of Chain Molecules", Interscience, New
York 1969.  Scheren P. A. G.M., Russell G. T., Sangster D. F,
Gilbert R. G., German A. L.: Macromolecules 1995, 28, 3637. 
Benson S. W., North A. M.: J. Am. Chem. Scoc. 1959, 81, 1339.
 Benson S. W., North A. M.: }. Am. Chem. Soc. 1962, 84, 935.
 North A. M., Reed G. A.: Trans. Faraday Soc. 1961, 57, 859.
 North A. M„ Reed G. A.: J. Polym. Sci. Ser. A 1969, 1, 1311.
 Mahabadi K. H„ O'Driscoll К. E: Macromolecules 1977, 10, 55.
 Mahabadi К. H., Rudin A.: ]. Polym. Sci. Polym. Chem. Ed.
1979,17,1801.  Bowman C. N., Peppas N. A.: Macromolecules 1991,
24, 914.  Goodner M. D., Bowman C.N. in: "Solvent-Free
Polymerizations and Processes" (eds., Lond T. E., Hunt M. O.), ACS
Symposium Series, No. 713, American Chemical Society, Washington,
DC, 1998, p. 220.  Horie, Otagawa A., Muraoka M., MitaJ.: }.
Polym. Sci. Polym. Chem. Ed. 1975, 13, 445.  NieJ., Linden L.
A., Rabek J. E, Fauassier J. R, Morlet-Sava- ry E, Scigalski E,
Wrzyszczyński A., Andrzejewska E.: Acta Polym. 1998, 49, 145. 
Andrzejewska E., An-
22 POLIMERY 2001, 46, nr 1
drzejewski M., Lindćn L. A., Rabek J. E: Polimen/ 1998, 43,
 Jakubiak J., Lindśn L. A., Rabek J. E: J. Polym. Sci.,
Polym. Chem. Ed. 2000, 38, 876.  Jakubiak J., Linden L. A.,
Rabek J. E: RadTech Europa '99, Berlin 1999, p. 417. 
Andrzejewska E., Lindśn L. A., Rabek J. E: Makromol. Chem. Phys.
1998, 199, 441.  Nie J., Andrzejewska E., Rabek J., Scigalski
E, Wrzyszczyński A.: Makromol. Chem. Phys. 1999, 200, 1692. 
Jakubiak J., Rabek J. E: Polimery 2000, 45, 485.  Schulz G.,
FischerJ.: }. Makromol. Chem. 1967, 107, 253.  Borgwardt U.,
Schnabel W., Henglein A.: Makromol. Chem. 1969, 127, 176. 
Yaraskavitch L, Brash ]., Hamielec A.: Polymer 1987, 28, 935. 
Zhu S., Hamielec A.: Macromolecules 1989, 22, 3093.  Li W.,
Hamielec A., Crowe C.: Polymer 1989, 30, 1513, 1518.
 Marten E, Hamielec A.: ]. Appl. Polym. Sci. 1982, 27, 489.
 Huguenin E G. E., Klein M. T.: Ind. Eng. Chem. Prod. Res.
Devel. 1985, 24, 166.  Batch G. L., Macosco C. W.: }. Appi.
Polym. Sci. 1992, 44, 1711.  Kurdikar D. L., Peppas N. A.:
Macromolecules 1994, 27, 4084.  Chiu W. Y., Carratt G. M.,
Soong D. S.: Macromolecules 1983, 16, 348.  O'Neil G. A.,
Wisnudel M. B., Torkelson J. M.: Macromolecules 1998, 31, 4537.
 Batch G. L., Macosco C. W.: SPE Antec 1987, 974.  Tulig T.
J., Tirrell M.: Macromolecules 1981, 14, 1501.  Rozenberg B.
A.: Adv. Polym. Sci. 1985, 75, 115.  Yu W., van Meerwall E. D.:
Macromolecules 1990, 23, 882.
 Sanford W. M., McCullough R. L.: J. Polym. Sci. Polym.
Phys. Ed. 1990, 28, 973.  Mita L, Horie K.: }. Macromol. Sci.
Rev. 1987, C27, 91.  Matsuoka S., Quan X., Bair H. E., Boyle D.
J.: Macromolecules 1989, 22, 4093.  Chiao L., Lyon R. E.: J.
Comp. Mat. 1990, 24, 739.  Cole K. C.: Macromolecules 1991, 24,
3093.  Shyichuk A. V.: ]. Appi. Polym. Sci. 1996, 61, 1703.
 Shechter L., Wynstra J., Kurkji R. P.: Ind. Eng. Chem. 1956,
48(1), 94.  Shyuchuk A. V., Lutsjak V. S.: Eur. Polym. J. 1995,
31, 631.  Dusek K., Somvarsky J. in: "Synthesis,
Characterization and Theory of Polymeric Networks and Gels" (ed.,
Aharoni S. M.), Plenum Press, New York 1992, p. 283.  Miller
D. R., Macosco C. W.: Macromolecules 1976, 9, 206.
 Macosko W., Miller D. R.: Macromolecules 1976, 9, 199.
 Scranton A. B., Klier J., Peppas N. A.: Macromolecules 1986,
19, 1412.  Williams R. J. J.: Macromolecules 1988, 21 , 2568.
 Williams R. J. J., Vallo C. L: Macromolecules 1988, 21, 2571.
 Dotson N. A., Galvan R., Macosko C. W.: Macromolecules 1988,
21, 2560.  Scranton A. B., Pappas N. A.: J. Polym. Sci., Chem.
Ed. 1990, 28, 99.  Mikos A. G., Takoudis C. G., Pep
pas N. A.: Macromolecules 1986, 19, 2174.  Mikos A.G. ,
Peppas N. A.: J. Contr. Release 1986, 5, 53.  ShuS., Hamielec
A. E.: Makromol. Chem. Macromol. Sym. 1988, 20/21, 501.  Mikos
A. G., Takeudis C. G., Peppas N. A.: Polymer 1987, 28, 998.
[Ill] Tobita H., Hamielec A. E.: Macromolecules 1989, 22, 3098.
 Zhu S., Hamielec A. E.: Macromolecules 1992, 25, 5457. 
Zhu S., Hamielec A. E.: Macromolecules 1993, 26, 3131.  Zhu
S., Hamielec A. E., PeltonR. H.: Makromol. Chem., Theory Simul.
1993, 2 , 587.  Pionka A., Paszkiewicz A.: }. Chem. Phys.
1992, 96,1128.  Manneville R, de Seze L.: "Numerical Methods
in the Study of Critical Phenomena", Springer Verlag, Berlin 1981.
 Hermann H. J., Landau D. P, Stauffer D.: Phys. Rev. Lett.
1982, 49, 412.  Bansil R., HarrmannH. J., Stauffer D.:
Macromolecules 1984, 17, 998.  Boots H. M. J., Pandey R. B.:
Polym. Bull. 1984, 11, 415.  Boots H. M. J., Klosterboer J.
G., van de Hei G. M. M.: Brit. Polym. J. 1985, 17, 219.
 Boots H. M. J., Dotson N.: Polym. Comm. 1988, 29, 346.
 Simon G. R, Allen R E. M., Bennet D. J., Williams D. R. G.,
Williams E. H.: Macromolecules 1989, 22, 3555.  Bowman C. N.,
Peppas N. A.: Chem. Eng. Sci. 1992, 47, 1411.  Kucybala Z.,
Pietrzak M., Paczkowski J., Linden L. A., Rabek J. E: Polymer 1996,
37, 4585.  Rabek J. E: in "Radiation Curing in Polymer Science
and Technology, Vol. I, Fundamentals and Methods" (eds., Fouasier
J. R, Rabek J. E), Elsevier Applied Science, London 1993, p. 453.
 Herlihy S.: Proc. Conf. RadTech '99, Berlin, Germany 1999, p.
489.  Sauerbrunn S., Armbruster D. A.: Proc. Conf. RadTech
'90, North America, Vol. 1, Chicago, Illinois, USA 1990, p. 303.
 Herlihy S., Battersby G. C.: Proc. RadTech '94 North America,
Florida, USA 1994, p. 156.  Sa- wada H.: }. Macromol. Sci.
1969, C3, 313.  AvramiM. : }. Chem. Phys. 1939, 7, 1103.
 Avrami M.: J. Chem. Phys. 1940, 8, 212.  Avrami M.:
J. Chem. Phys. 1941, 9, 117.  Waters D.N. , Paddy J. L.: Anal.
Chem. 1988, 60, 53.  Tedder J. M. in: "Reactivity, Mechanism
and Structure in Polymer Chemistry" (eds., Jenkins A. D., Ledwith
A.), Wiley, New York 1974.  Moad G., Solomon D. H.: "The
Chemistry of Free Radical Polymerization", Pergamon, London 1995.
 Mateo J. L., Bosch R, Lozano A. E.: Macromolecules 1994, 27,
7794.  Hammett L. R: /. Am. Chem. Soc. 1937, 59, 96. 
Connors K. A.: "Chemical Kinetics", VCH Publisher, Weinheim 1990,
Received 7 XII 1999.